dynamics, in organic molecular crystals lattice phonons are the fingerprints of the indi-vidual crystal structure. Typical examples of the application of Raman spectroscopy to polymorphism in organics are pentacene [42, 43], tetracene  and α-sexithiophene .
Fig. 4.3 shows the identification of the two polymorphs of pentacene and α-sexithiophene by means of their lattice phonons spectra.
Figure 4.3: Lattice phonons Raman spectra of the two polymorphic form of pentacene and α-sexithiophene and their corresponding crystal structures.
The physical purity (phase homogeneity) of a crystal is directly related to crystal phase identification. Different crystal phases can coexist as different domains in the same crystallite, originating a phase mixing which ultimately affects the physical purity of the sample . The use of an optical microscope coupled to the Raman spectrometer and making the microscope confocal allows the scaling down in size of the crystal region under investigation. Raman scattering is transmitted to the spectrometer only from the restricted sampling volume determined by the focused region of the laser beam, enabling fine tuning of XYZ discrimination. Spatial resolution down to 1 µm and less can be easily achieved. The problem of phase mixing is well known in thin films [46, 47], and is one
of the reasons of the difficulties in obtaining reliable structural characterization. This problem is relevant also for single crystals and a typical example is shown in Fig. 4.4.
Once the spectral profiles of the single polymorphs are identified by lattice phonon Raman spectroscopy, they are used as reference spectra and it is easy to monitor physical impurities in which domains of one polymorph embedded inside the other. As reported
Figure 4.4: Examples of phase mixing in crystalline pentacene and α-sexithiophene.
in Fig. 4.4 for crystalline samples of pentacene and α-sexithiophene, the coexistence of phases appears as an overlap of distinctive phonon bands of either polymorph in the same crystal grain (green traces), as indicated by the vertical bars with reference to the pure polymorph spectra. Phase mixing, or physical inhomogeneities, is observed in most cases where polymorphism occurs [42, 44], demonstrating the general validity and the sensitivity of this technique for detecting the presence of domains of either structure at the µm scale.
It is of great importance to find a suitable method for checking phase homogeneity in each crystal domain by obtaining a visual display of the physical purity. This task can be nicely fulfilled by confocal Raman mapping (CRM) in the region of lattice phonons (10-150 cm−1), outlining a further application of confocality to micro-spectrometry tech-niques. By scanning the surface, typically few tens of mm wide, with steps as close as 1 µm, one can obtain a series of Raman spectra which can be collected, point by point, in an actual map to be compared to the optical image of the original sample [65, 48], as schematically shown in Fig. 4.5. This will yield crucial information on the topography of each crystal whose phase homogeneity needs to be checked. The spatial resolution is given by the laser spot area and is ranging from 0.88 to 1.05 µm, depending on the numerical aperture of the microscope objective and on the wavelength of the laser line.
Figure 4.5: Scheme of a confocal Raman mapping experiment.
The actual recipe of the lattice phonon CRM technique can be summarized in four steps:
1. Assign spectra to structures;
2. Scan selected crystal regions;
3. Identify phase mixing;
4. Map structural homogeneity.
The first step requires a careful micro-Raman investigation of a large number of crys-talline samples grown in as many conditions as possible, to search for all possible poly-morphs. This will yield a series of “reference spectra”, each corresponding to a distinct polymorph. This also enables one to select suitable wavenumber windows typical of each crystal phase. The second step concerns the choice of the specimen regions to be investi-gated, planning a number of point spectra sufficient to reconstruct spectroscopically the sample with a good spatial resolution. In the following step the identification of phase mixing is achieved by comparing complex spectral profiles with the reference spectra of the pure polymorphs. The final step eventually yields the phase Raman mapping of the selected crystal domain, which is obtained by monitoring the spectral windows where either one or the other polymorph shows phonon bands. The relative amount of one phase with respect to the other can therefore be quantitatively represented by the intensity ratio of selected bands and at once converted, with a suitable software, in a conventional palette of colours. For instance, when both A and B forms are present, one can represent the intensity ratio A/B by adopting a blue-green color for the A
phase, while the red-yellow shades correspond to an increasing amount of B phase. A deconvolution of the phonon bands with background suppression will assure a reliable representation of the data. The spread of colors indicates the extent of the phase mix-ing between the two polymorphs analyzed in the chosen crystal domain. Phase purity obviously is obtained when the overall color remains virtually homogeneous throughout the whole surface scanned. Phase mixing is instead represented by a different extent of one phase inside the other and produces marked differences in the color conventionally chosen as reference of either polymorph. Examples of lattice phonon CRM are given
Figure 4.6: Optical (left) and Raman (right) images of selected pentacene crystals.
Raman mapping refers to the area XY (µm2) drawn as a box over the optical image of the crystal. In the Raman maps the color drifts from blue (full H phase) to green/red (increasing amount of C phase). The color scale is selected each time to emphasize the phase mixing in the crystal grain (from ).
in Fig. 4.6 and Fig. 4.7 for pentacene and α-sexithiophene, respectively. A variety of situations is observed in pentacene which shows a different extent of phase mixing in three selected crystals whose optical images are otherwise homogeneous. Pentacene was the very first example of an organic material mapped with this technique . In the case of α-sexithiophene the sample in the lowest part of the Fig. 4.7 is a nice example of phase purity, showing a full homogeneous colour, in spite of a large expansion of the conventional color scale. Phase mixing is instead represented by a different extent of one phase inside the other and produces differences in the colour maps, as shown for
Figure 4.7: Optical images (left) and Raman maps (right) of α-sexithiophene crystalline samples exhibiting phase inhomogeneity. Raman mapping refers to the area XY (µm2) drawn as a box over the optical picture of the crystal. In the Raman maps the colour drifts from blue-green (LT phase) to red-yellow (increasing amount of HT phase). The colour scale is selected each time to emphasize the phase mixing in each crystal grain (from ).
the other two specimens (top and middle sets of Fig. 4.7). As expected, the contours of the optical images are nicely reproduced in the corresponding Raman maps, yielding direct information on which crystal phase is present and in what extent. Furthermore, the comparison between the optical images and the Raman maps show with clear ev-idence that no relationship exists between morphology and crystal phase: structural information and phase mixing can be efficiently monitored only by Raman maps. It is then crucial to perform a spectroscopic test in order to verify the phase purity in all crystals treated, especially for those cases in which crystal morphology cannot assist phase recognition. It is thus conclusively shown that lattice phonon CRM is a most efficient tool to identify polymorphs and their mixing in the same crystallite at a µm scale. An additional feature related to the confocality of the micro-Raman technique concerns with the possibility to probe phase homogeneity of crystal domains at different sample depths [65, 48]. This is illustrated in Fig. 4.8, where lattice phonon Raman spectra, taken on the very same spot in a given crystal domain, show a variation of the relative amount of either polymorph on penetrating inside the bulk. This is achieved by probing the sample surface at different penetration depths by focusing the laser light
Figure 4.8: An example of Raman phonon spectra of α-sexithiophene taken with differ-ent microscope objectives, as labeled. The penetration depth increases from the bottom to the top spectra (in black) of the figure. For better reference, HT and LT lattice phonon spectra are also reported.
with microscope objectives having different numerical apertures. Typical values of the theoretical penetration depths vary from 7.5 µm (100x) to 25 µm (50x) up to a depth of about 450 µm (10x). On getting into the bulk, different amount of phase mixing is found, with an increase of the fraction of LT polymorph, as indicated by the vertical lines that monitor both phases with their reference phonon. It is then important to re-mark that phase inhomogeneity is not confined to the first layers of the crystal surface, but it propagates into the bulk. The possibility of a three dimensional investigation of single crystal homogeneity is thus an additional appealing feature of this technique applied to heterogeneous solid phases.